1 Construction Analysis SGS-Thomson M28C K EEPROM Report Number: SCA Global Semiconductor Industry the Serving Since N. Hartford Drive Scottsdale, AZ Phone: Fax: Internet:
2 INDEX TO TEXT TITLE PAGE INTRODUCTION 1 MAJOR FINDINGS 1 TECHNOLOGY DESCRIPTION Assembly 2 Die Process and Design 2-3 ANALYSIS RESULTS I Assembly 4 ANALYSIS RESULTS II Die Process and Design 5-6 TABLES Procedure 7 Overall Quality Evaluation 8 Package Markings 9 Wirebond Strength 9 Die Material Analysis 9 Horizontal Dimensions 10 Vertical Dimensions 10
3 INTRODUCTION This report describes a construction analysis of the SGS-Thomson M28C K EEPROM. Five devices packaged in 28-pin Dual In-Line Packages (DIPs) were received for the analysis. Devices were date coded MAJOR FINDINGS Questionable Items: 1 None. Special Features: None. 1 These items present possible quality or reliability concerns. They should be discussed with the manufacturer to determine their possible impact on the intended application
4 TECHNOLOGY DESCRIPTION Assembly: Devices were packaged in 28-pin Dual In-Line Packages (DIPs). Lead-locking provisions (holes and anchors) at all pins. Wirebonding was by the thermosonic ball bond method using 1.2 mil O.D. gold wire. All pins except pin 26 were connected. No multiple bonding wires were noted. Die separation was by sawing (full depth). Silver-filled epoxy die attach. Die Process : Devices were fabricated using a selective oxidation, N-well CMOS process in a P substrate. No epi was used. No die coat was present. Passivation consisted of two layers of silicon-dioxide (probably undoped). Metallization consisted of a single layer of dry-etched aluminum. The aluminum contained a titanium-nitride cap and barrier. There appeared to be a thin layer of titanium-aluminum (TiAl) precipitate or titanium (Ti) above the barrier (see Figure 11). A thin titanium adhesion layer was used under the barrier. Standard contacts were used (no plugs)
5 TECHNOLOGY DESCRIPTION (continued) Pre-metal dielectric consisted of a layer of CVD glass (probably BPSG) over various densified oxides. The glass appeared to be reflowed following contact cuts. A single layer of dry-etched polycide (poly and tungsten silicide) was used. This layer formed all gates on the die, and in the cell array it formed the capacitors, word lines, and tunnel oxide device. Standard implanted N+ and P+ diffusions formed the sources/drains of the MOS transistors. An LDD process was used with oxide sidewall spacers left in place. Local oxide (LOCOS) isolation. No step was present at the edge of the well boundaries. The memory cell consisted of a standard EEPROM design. Metal was used to form the bit lines. Poly was used to form the word/select lines, capacitors, and the tunnel oxide devices. Redundancy fuses were not present
6 ANALYSIS RESULTS I Package and Assembly: Figures 1-5 Questionable Items: 1 None. Special Features: None. General Items: Devices were packaged in 28-pin Dual In-Line Packages (DIPs). Overall package quality: Good. No defects were noted externally or internally on the package. All pins were well formed. Lead-locking provisions (anchors and holes) were present. Wirebonding was by the thermosonic ball bond method using 1.2 mil O.D. gold wire. The clearance of the wires was normal. Bond pull strengths were normal (see page 9). No problems were noted. Die attach: A silver-epoxy was used to attach the die to the header. No significant voids were noted. Die dicing: Die separation was by sawing of normal quality. No large cracks or chips were present. 1 These items present possible quality or reliability concerns. They should be discussed with the manufacturer to determine their possible impact on the intended application
7 ANALYSIS RESULTS II Die Process: Figures 6-26 Questionable Items: 1 None. Special Features: None. General Items: Fabrication process: Devices were fabricated using a selective oxidation, N-well CMOS process in a P substrate. No epi was used. Process implementation: Die layout was clean and efficient. Alignment was good at all levels. No damage or contamination was found. Die coat: No die coat was present. Overlay passivation: The passivation consisted of two layers of silicon-dioxide (probably undoped). Overlay integrity test indicated defect-free passivation. Edge seal was good. Metallization: A single layer of metal consisting of aluminum with a titanium-nitride cap and barrier. There appeared to be a thin layer of titanium-aluminum (TiAl) precipitate or titanium (Ti) above the barrier. A thin titanium adhesion layer was used under the barrier. Standard contacts were used (no plugs). No problems were noted. Metal patterning: The metal layer was patterned by a dry etch of normal quality. Contacts were completely surrounded by metal and metal lines were widened at contacts. Metal defects: No voiding, notching, or neckdown was noted in the metal layer. 1 These items present possible quality or reliability concerns. They should be discussed with the manufacturer to determine their possible impact on the intended application
8 ANALYSIS RESULTS II (continued) Metal step coverage: Aluminum thinned up to 60 percent at contact edges. Total metal thinning was reduced to 40 percent with the addition of the cap and barrier. MIL-STD allows up to 70 percent metal thinning for contacts of this size. Pre-metal dielectric: A layer of CVD glass (probably BPSG) over various densified oxides was used under the metal. Reflow appeared to be performed following contact cuts. No problems were found. Contact defects: None. Contact cuts were well rounded. No over-etching of the contacts was noted. Polysilicon: A single layer of polycide (poly and tungsten silicide) was used to form all the gates on the die and in the cell. The poly formed the word/select lines, capacitors, and the tunnel oxide device. Diffusions: Standard implanted N+ and P+ diffusions formed the sources/drains of the MOS transistors. An LDD process was used with oxide sidewall spacers left in place. Diffusions were not silicided. No problems were noted. Isolation: Local oxide (LOCOS) isolation was used. No step was present in the oxide at the well boundary. EEPROM array: Memory cell consisted of a standard EEPROM design. Metal was used to form the bit lines. Poly was used to form the word/select lines, capacitors, and the tunnel oxide device. Cell pitch was 7.8 x 15.0 microns. Redundancy fuses were not present on the die
9 PROCEDURE The devices were subjected to the following analysis procedures: External inspection X-ray Decapsulation Internal optical inspection SEM of passivation Passivation integrity test Wirepull test Passivation removal SEM inspection of metal Metal removal and inspect barrier Delayer to silicon and inspect poly/die surface Die sectioning (90 for SEM) * Die material analysis (EDX) Measure horizontal dimensions Measure vertical dimensions * Delineation of cross-sections is by silicon etch unless otherwise indicated
10 OVERALL QUALITY EVALUATION: Overall Rating: Normal/Good DETAIL OF EVALUATION Package integrity Package markings Die placement Wirebond placement Wire spacing Wirebond quality Die attach quality Dicing quality Die attach method Dicing method Wirebond method N N N N N N N N Silver epoxy Sawn (full depth) Thermosonic ball bonds using 1.2 mil gold wire. Die surface integrity: Toolmarks (absence) Particles (absence) Contamination (absence) Process defects (absence) General workmanship Passivation integrity Metal definition Metal integrity Contact coverage Contact registration G G G G G G N N G G G = Good, P = Poor, N = Normal, NP = Normal/Poor - 8 -
11 PACKAGE MARKINGS (TOP) (LOGO) M28C H8AA627F KOREA BOTTOM XOP641FA M WIREBOND STRENGTH Wire material: Die pad material: 1.2 mil O.D. gold Aluminum Sample # 1 # of wires pulled: 9 Bond lifts: 0 Force to break - high: 15g - low 14g - avg. 14.5g - std. dev.: 0.5 DIE MATERIAL ANALYSIS (EDX) Overlay passivation: Metallization: Poly: A layer of nitride over a layer of silicondioxide. Aluminum (Al) with a titanium-nitride (TiN) cap and barrier. There appeared to be a layer of titaniumaluminum (TiAl) precipitate or titanium (Ti) above the barrier. A thin layer of titanium (Ti) was used under the barrier. Tungsten (W) silicide
12 HORIZONTAL DIMENSIONS Die size: 3.2 x 6.7 mm (125 x 265 mils) Die area: 21.5 mm 2 (33,125 mils 2 ) Min pad size: 0.11 x 0.11 mm (4.5 x 4.5 mils) Min pad window: 0.09 x 0.09 mm (3.8 x 3.8 mils) Min pad space: 3.0 mils Min metal width: 1.0 micron Min metal space: 1.4 micron Min metal pitch: 2.4 microns Min contact: 0.8 micron Min polycide width: 1.2 micron Min polycide space: 1.1 micron Min gate length - (N-channel): * 1.2 micron - (P-channel): 1.3 micron Cell pitch: 7.8 x 15.0 microns Cell size: microns VERTICAL DIMENSIONS Die thickness: 0.5 mm (20 mils) Layers: Passivation 2: 0.65 micron Passivation 1: 0.35 micron Metal - cap: 0.07 micron (approximate) - aluminum: 0.65 micron - barrier: 0.15 micron Pre-metal dielectric: 0.65 micron (average) Oxide on poly: 0.15 micron Poly - silicide: 0.15 micron - poly: 0.15 micron Local oxide: 0.55 micron N+ S/D: 0.25 micron P + S/D: 0.4 micron N-well: 4.0 microns (approximate) * Physical gate length
13 INDEX TO FIGURES PACKAGE ASSEMBLY Figures 1-5 DIE LAYOUT AND IDENTIFICATION Figures 6-8 PHYSICAL DIE STRUCTURES Figures 9-26 COLOR PROCESS DRAWING Figure 20 MEMORY CELL Figures CIRCUIT LAYOUT AND I/O STRUCTURE Figure 26
14 RB 1 28 V CC A W A N.C. top A6 A A8 A9 A A11 A G A A10 A E A DQ7 DQ DQ6 DQ DQ5 DQ DQ4 VSS DQ3 bottom Figure 1. Package photographs and pinout of the SGS-Thomson M28C EEPROM. Mag. 2.5x.
15 PIN top side Figure 2. X-ray views of the package. Mag. 2.5x.
16 Ag EPOXY Mag. 250x EDGE OF PASSIVATION Mag. 1300x Figure 3. Perspective SEM views of dicing and edge seal. 60.
17 EDGE OF PASSIVATION EDGE OF DIE Mag. 1600x PASSIVATION METAL DIFFUSION Mag. 6500x Figure 4. SEM section views of the edge seal.
18 Mag. 550x, 60 Au BOND PAD Au Mag. 810x Au Mag. 6500x PASSIVATION METAL 2 BOND PAD Figure 5. SEM views of typical ball bonds.
19 Figure 6. Whole die photograph of the M28C EEPROM. Mag. 34x.
20 Mag. 320x Mag. 400x Figure 7. Optical views of markings on the die surface.
21 Figure 8. Optical views of the die corners. Mag. 160x.
22 PASSIVATION METAL POLY glass-etch PASSIVATION METAL POLY P+ DIFFUSIONS silicon-etch Figure 9. SEM section views of general circuitry. Mag. 13,000x.
24 PASSIVATION 2 PASSIVATION 1 ALUMINUM PRE-METAL DIELECTRIC Mag. 26,000x PASSIVATION 2 PASSIVATION 1 TiN CAP ALUMINUM TiN BARRIER Ti ADHESION LAYER Mag. 40,000x Figure 11. SEM section views of metal line profiles.
25 CONTACT METAL Mag. 4400x CONTACT METAL Mag. 7700x Figure 12. Topological SEM views illustrating metal patterning. 0.
26 METAL Mag. 6500x TiN CAP ALUMINUM Mag. 13,000x TiN BARRIER TiN BARRIER Mag. 20,000x Figure 13. SEM views illustrating metal step coverage and barrier coverage. 60.
27 PASSIVATION METAL metal 1-to-poly PRE-METAL DIELECTRIC POLY TiN CAP ALUMINUM TiN BARRIER POLY metal 1-to-P+ P+ DIFFUSION TiN CAP metal 1-to-N+ TiN BARRIER ALUMINUM N+ DIFFUSION Figure 14. SEM section views of metal contacts (silicon etch). Mag. 26,000x.
28 POLY Mag. 3200x GATES POLY DIFFUSION Mag. 6500x Figure 15. Topological SEM views of poly patterning. 0.
29 POLY POLY GATES Mag. 3200x POLY Mag. 40,000x LOCAL OXIDE POLY Mag. 40,000x LOCAL OXIDE Figure 16. Perspective SEM views of poly coverage. 60.
31 PRE-METAL DIELECTRIC OXIDE ON POLY SILICIDE LOCAL OXIDE POLY GATE OXIDE Figure 18. SEM section view of a typical local oxide birdsbeak. Mag. 40,000x. N-WELL P SUBSTRATE Figure 19. Optical section view illustrating the well structure. Mag. 800x.
32 CAP BARRIER SGS-Thomson M28C64-121,,,,,,,,,,,,,,,,,,,, ALUMINUM N+ S/D PASSIVATION 2 PASSIVATION 1 PRE-METAL DIELECTRIC LOCAL OXIDE P SUBSTRATE P+ S/D SILIICIDE POLY N-WELL Orange = Nitride, Blue = Metal, Yellow = Oxide, Green = Poly, Red = Diffusion, and Gray = Substrate Figure 20. Color cross section drawing illustrating device structure.
33 metal 1 poly Figure 21. Perspective SEM views of the EEPROM cell array. Mag. 3200x, 60.
34 metal 1 B BIT LINE A WORD TUNNEL OXIDE DEVICE poly 3 C 2 G 1 WORD SHARED WITH ADJACENT CELL BIT A 1 G (TO ADJACENT CELL) 2 C 3 BIT B Figure 22. Topological SEM views and schematic of the EEPROM cell. Mag. 3200x, 0.
35 PASSIVATION METAL BIT LINE Mag. 6500x DIFFUSION WORD/SELECT CAPACITOR PLATE TUNNEL OXIDE DEVICE METAL BIT LINE Mag. 13,000x WORD/SELECT N+ DIFFUSION METAL PRE-METAL DIELECTRIC POLY Mag. 26,000x TUNNEL OXIDE WINDOW DELINEATION ARTIFACT Figure 23. SEM section views of the EEPROM cell (parallel to bit line).
36 PASSIVATION BIT LINE METAL TUNNEL OXIDE DEVICE POLY GATE (2) N+ Mag. 6500x POLY TUNNEL OXIDE Mag. 52,000x Figure 24. SEM section views of the EEPROM cell (perpendicular to bit lines).
37 PASSIVATION METAL BIT LINE LOCAL OXIDE N+ DIFFUSION Mag. 10,000x METAL BIT LINE N+ DIFFUSION Mag. 26,000x Figure 25. SEM section views of the EEPROM cell (perpendicular to bit line).
38 Mag. 200x Mag. 800x Figure 26. Optical views of an I/O structure and general circuitry.